#------------------------------------------------------------------------------
#$Date: 2022-09-15 03:04:42 +0300 (Thu, 15 Sep 2022) $
#$Revision: 277859 $
#$URL: file:///home/coder/svn-repositories/cod/cif/4/30/05/4300556.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4300556
loop_
_publ_author_name
'Dikarev, Evgeny V.'
'Filatov, Alexander S.'
'Clerac, Rodolphe'
'Petrukhina, Marina A.'
_publ_section_title
;
Unligated Diruthenium(II,II) Tetra(trifluoroacetate): The First X-Ray 
Structural Study, Thermal Compressibility, Lewis Acidity and Magnetism
;
_journal_issue                   2
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              744
_journal_page_last               751
_journal_paper_doi               10.1021/ic051537m
_journal_volume                  45
_journal_year                    2006
_chemical_formula_moiety         'Ru2 (O2 C C F3)4'
_chemical_formula_sum            'C8 F12 O8 Ru2'
_chemical_formula_weight         654.22
_chemical_melting_point          'not measuerd'
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                80.6060(10)
_cell_angle_beta                 85.3370(10)
_cell_angle_gamma                86.985(2)
_cell_formula_units_Z            1
_cell_length_a                   5.2519(5)
_cell_length_b                   8.6122(8)
_cell_length_c                   9.3269(9)
_cell_measurement_temperature    243(2)
_cell_volume                     414.49(7)
_diffrn_ambient_temperature      243(2)
_exptl_crystal_density_diffrn    2.621
_cod_database_code               4300556
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Ru1 Ru 0.18233(5) 0.46436(3) 0.55580(3) 0.02722(13) Uani 1 1 d . . .
O1 O 0.3916(5) 0.5811(3) 0.3741(3) 0.0323(6) Uani 1 1 d . . .
O2 O 0.2162(5) 0.2642(3) 0.4614(3) 0.0361(6) Uani 1 1 d . . .
O4 O 0.1462(5) 0.6652(3) 0.6490(3) 0.0366(6) Uani 1 1 d . . .
O3 O -0.0291(5) 0.3504(4) 0.7328(3) 0.0352(6) Uani 1 1 d . . .
F5 F 0.2094(7) -0.0145(3) 0.3751(4) 0.0623(8) Uani 1 1 d . . .
F6 F -0.1394(8) 0.0490(4) 0.2768(4) 0.0775(10) Uani 1 1 d . . .
C2 C 0.0467(7) 0.2464(5) 0.3792(4) 0.0350(8) Uani 1 1 d . . .
C1 C 0.2660(7) 0.6452(4) 0.2688(4) 0.0322(8) Uani 1 1 d . . .
F4 F 0.2112(9) 0.1436(4) 0.1742(4) 0.0939(14) Uani 1 1 d . . .
C4 C 0.0831(10) 0.1031(6) 0.2996(5) 0.0486(11) Uani 1 1 d . . .
C3 C 0.4187(8) 0.7225(6) 0.1321(5) 0.0445(10) Uani 1 1 d D A 1
F1 F 0.2769(14) 0.7900(13) 0.0264(8) 0.0315(16) Uiso 0.33 1 d PD A 1
F2 F 0.5651(18) 0.8348(11) 0.1735(10) 0.0255(18) Uiso 0.33 1 d PD A 1
F3 F 0.579(3) 0.6151(12) 0.0807(16) 0.035(3) Uiso 0.33 1 d PD A 1
F1X F 0.2644(17) 0.8420(12) 0.0538(10) 0.050(3) Uiso 0.33 1 d PD A 2
F2X F 0.603(2) 0.8065(15) 0.1571(16) 0.065(5) Uiso 0.33 1 d PD A 2
F3X F 0.497(3) 0.6254(17) 0.0471(16) 0.108(7) Uiso 0.33 1 d PD A 2
F1Y F 0.2845(19) 0.7253(15) 0.0085(10) 0.061(3) Uiso 0.33 1 d PD A 3
F2Y F 0.514(3) 0.8540(13) 0.1305(17) 0.082(4) Uiso 0.33 1 d PD A 3
F3Y F 0.614(3) 0.6194(18) 0.0974(18) 0.070(7) Uiso 0.33 1 d PD A 3
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Ru1 O3 2.051(3) . y
Ru1 O4 2.053(3) . y
Ru1 O2 2.053(3) . y
Ru1 O1 2.085(3) . y
Ru1 Ru1 2.2627(5) 2_566 y
Ru1 O1 2.377(3) 2_666 y
O1 C1 1.262(5) . n
O1 Ru1 2.377(3) 2_666 n
O2 C2 1.252(5) . n
O4 C2 1.254(5) 2_566 n
O3 C1 1.244(4) 2_566 n
F5 C4 1.317(6) . n
F6 C4 1.326(6) . n
C2 O4 1.254(5) 2_566 n
C2 C4 1.537(6) . n
C1 O3 1.244(4) 2_566 n
C1 C3 1.525(5) . n
F4 C4 1.306(5) . n
C3 F1 1.323(8) . n
C3 F3 1.339(9) . n
C3 F2 1.388(8) . n
